**RATCHET LIMITS FOR A CRACK IN A WELDED PIPE SUBJECTED TO A CYCLIC **

**TEMPERATURE LOAD AND A CONSTANT MECHANICAL LOAD **

** Tianbai Li Haofeng Chen **

Department of Mechanical Engineering Department of Mechanical Engineering University of Strathclyde University of Strathclyde

### Glasgow, Scotland, UK Glasgow, Scotland, UK

** ** ** Weihang Chen James Ure **

Department of Mechanical Engineering Department of Mechanical Engineering ** **

University of Strathclyde University of Strathclyde

### Glasgow, Scotland, UK Glasgow, Scotland, UK

**ABSTRACT **

This paper presents the ratchet limit analysis of a pipe with a symmetric crack in a mismatched weld by using the extended Linear Matching Method (LMM). Two loading conditions are considered: i) a cyclic temperature load and a constant internal pressure; and ii) a cyclic temperature load and a constant axial tension. Individual effects of i) the geometry of the Weld Metal (WM), ii) the size of the crack, iii) the location of the crack and iv) the yield stress of WM on the ratchet limits, maximum temperature ranges to avoid ratchetting and limit loads are investigated. Influence functions of the yield stress of WM on the maximum temperature ranges and limit loads are generated. The results confirm the applicability of the extended LMM to the cracked welded pipe.

*Keywords: crack, ratchet limit, limit load, welded pipe, *
*maximum temperature range *

**INTRODUCTION **

The circumferential butt welded pipes are widely used in nuclear power plants and usually subjected to complex varying thermal and mechanical loads [1-2]. Under such loads, the pipes may fail either from the accumulated plastic deformations during the increasing load cycles or from the reverse plastic deformations. The former is known as ratchetting, which leads structures to incremental collapse; the latter is named plastic shakedown, which gives rise to local low cycle fatigue. For a pipe with a crack in the weld, the elastic stress singularity at the crack tip violates the elastic shakedown condition, hence the non-existence of a finite shakedown limit. Therefore the ability to calculate the ratchet limit of the cracked pipe is particularly desirable. The obtained ratchet limit may then be used to calculate the ratchetting reference stress to predict material deformation and rupture [3].

Ratchetting analysis of loaded structures has been investigated by many researchers in past decades [2-20]. The complexity of ratchetting means that analytical solutions are rare, and thus incremental Finite Element Analysis (FEA) is widely used. Incremental FEA can only show if ratchetting occurs, and therefore many calculations are required to generate the Bree-like diagram [4].

In order to overcome the difficulties of the step-by-step elasto-plastic FEA, a number of direct methods based upon the Koiter's [5] kinematic and/or the Melan's [6] static theorems have been developed including: i) the nonlinear superposition method [7]; ii) mathematical programming methods [8-9]; iii) the Generalized Local Stress Strain (GLOSS) r-node method [10]; iv) the Elastic Compensation Method (ECM) [11, 12]; and v) the Linear Matching Method (LMM) [13-20]. The LMM is distinguished from other simplified methods by ensuring that equilibrium and compatibility are satisfied at each stage. The LMM has been shown to give accurate shakedown analysis to complex geometries and load histories [13, 14]. The LMM has also been extended to evaluate ratchet limits [15-18] for defect-free components subjected to cyclic load conditions from two-load extremes [15-17] to multi-two-load extremes [18]. However, the application of the latest LMM ratchet limit method [18] to structures with a discontinuity in the geometry and material has not yet been undertaken.

location and size of the crack, width of the WM, and finally the coefficient of thermal expansion of the WM on the ratchet limit are discussed.

**LINEAR MATCHING METHOD **

Consider a body of volume, *V*, with a surface area *S*. The

body is subjected to varying mechanical loads, *P* (*xi*,*t*)

*V*

, over a

fraction of the surface area, *Sp*, and varying thermal loads

)
,
(*xi* *t*
*V*

θ . A zero displacement rate condition is applied over

the remainder of the surface area, *Su* such that *u*&*i* =0. Over a

time cycle 0≤*t*≤Δ*t*, these loads are decomposed into constant

and cyclic components such that

) , ( ) ( ) ,

(*x* *t* *P* *x* *P* *x* *t*

*P* *i* *i* *i*

*v* =λ +

, θ*v*(*x _{i}*,

*t*)=λθ(

*x*)+θ(

_{i}*x*,

_{i}*t*)

(1)

where λ is a load multiplier. *P* and θ are the constant

mechanical and thermal load distribution respectively. *P*and

θ are the cyclic mechanical and thermal load respectively. The

corresponding linear elastic stress history σˆ is then given as *ij*

ˆ (*x* ,*t*) (*x* ) ˆ (*xk*,*t*) ˆ*ij*(*xk*,*t*)

*P*
*ij*
*k*
*ij*
*k*
*ij*
θ
σ
σ
σ
λ

σ = + + (2)

where σ*ij*(*xk*)is the elastic stress due to *P*and θ . ˆ (*xk*,*t*)
*P*
*ij*
σ

and ˆ*ij*(*xk*,*t*)

θ

σ are the elastic stress histories corresponding to

)
,
(*x* *t*

*P* * _{k}* and θ(

*xk*,

*t*), respectively. The cyclic stress history

)
,
(*xk* *t*
*ij*

σ over the time cycle is given by

(*x* ,*t*) ˆ (*x* ,*t*) (*x* ) *r*(*x _{k}*,

*t*)

*ij*
*k*
*ij*
*k*
*ij*
*k*

*ij* σ ρ ρ

σ = + + (3)

where ρ*ij*(*xk*) is a constant residual stress and corresponds to

)
( _{k}*ij* *x*
σ

λ . *r*(*x _{k}*,

*t*)

*ij*

ρ is a changing residual stress corresponding

to *P*

*ij*

σˆ and σˆ*ij*θduring a cycle and satisfies:

)
(
)
,
(
)
0
,
( 0
*k*
*ij*
*k*
*r*
*ij*
*k*
*r*

*ij* *x* ρ *x* *t* ρ *x*

ρ = Δ = (4)

where 0( )

*k*
*ij* *x*

ρ is the constant element of *r*

*ij*
ρ

Consider an energy function

*I* *cdtdV*

*ij*
*V*
*t*
*ij*
*c*
*ij*
*c*

*ij* λ σ σ ε

ε& =∫ ∫Δ − &

0

) (

) ,

( (5)

where *c*

*ij*

ε& is a kinematically admissible strain rate. *c*
*ij*
σ

represents a stress at yield corresponding to *c*

*ij*
ε& .

The determination of the ratchet limit is implemented by a two-stage nonlinear minimisation procedure: i) a changing

residual stress *r*

*ij*

ρ is computed by an incremental minimisation

of the energy function *I* and satisfies Eq. (4), with the

application of the cyclic load; and ii) a global minimisation of the upper bound shakedown theorem is performed to evaluate the additional constant load, which leads the load state to the ratchet limit.

Consider a body subjected to a cyclic load involving multi-load extremes. It is assumed that plastic strains only occur at

the extremes corresponding to the time instants *tk*(*k*=1,...,*K*).

The instants *tk* represents a sequence of time points in the

cyclic load history such that Δ =∑ Δ

=
*K*
*k* *k*
*p*
*ij*
*c*
*ij* *t*
1
)
(
ε

ε , where

)
(_{k}*p*
*ij* *t*
ε

Δ is the plastic strain increment at *tk*. Hence we have the

function

*I* *I* *t* *t* *kdV*

*ij*
*k*
*r*
*ij*
*k*
*ij*
*V*
*K*
*k*
*k*
*ij*
*K*
*k* *k*
*c*

*ij* λ σ σ ρ ε

ε =∑ =∫ ∑ − − Δ

= = ( ) ( )) ˆ ( ) , ( 1 1

& (6)

where

= +∑ Δ

=
*k*

*m* *ij* *m*
*ij*

*k*
*r*

*ij* *t* *t*

1

0 _{(} _{)}

)

( ρ ρ

ρ (7)

( ) ( ) ( ) *p*(* _{k}*)

*ij*
*k*
*mn*
*k*
*ijmn*
*k*
*T*

*ij* *t* *C* μ ρ *t* ε *t*

ε = Δ +Δ

Δ (8)

) 2 /( ) ) ( ) ( ˆ ) ( ˆ ( )

( *r* _{k}_{k}

*ij*
*k*
*ij*
*k*
*P*
*ij*
*k*
*p*

*ij* *t* σ *t* σ *t* ρ *t* μ

ε _{=} _{+} θ _{+} _{′}

Δ (9)

where *T*

*ij*
ε

Δ is compatible and Δρ*ij* satisfies equilibrium. An

upper 'dash' refers to deviatoric components. μ*k*is an iterative

shear modulus and determined by the linear matching condition [15,16]

3 ( ( ))

2
*k*
*p*
*ij*
*y*
*k*
*t*

### ε

### ε

### σ

### μ

Δ= _{ (10) }

where σ*y* is the yield stress and ( (*k*))

*p*
*ij* *t*
ε

ε Δ is the effective

plastic strain increment.

The changing residual stress is computed by the

minimisation of the *I*via the iterations among Eqs. (7-10). We

denote *n*(* _{k}*)

*ij* *t*
ρ

Δ as an evaluated changing residual stress at

*th*

*k* load instance after *th*

*n* iteration, where *k*=1,...,*K* and

*N*
*n*=1,..., . At _{n}th

iteration, (*k*)

*n*
*ij* *t*
ρ

Δ is computed for all *K*load

instances. The converged solution occurs if the summation of

all changing residual stresses at *th*

*N* iteration vanishes, i.e.

0
)
(
1
=
∑ Δ
= *k*
*K*
*k*
*N*
*ij* *t*

ρ . Hence the constant residual stress 0

*ij*

ρ can also

be determined by

=∑ ∑ Δ

= =
*K*
*k*
*N*
*n* *k*
*n*
*ij*
*ij* *t*
1 1
0
)
(
ρ

ρ (11)

The ratchet limit can be determined by the minimisation of the upper bound shakedown theorem [15], with the elastic

solution augmented by the changing residual stress *r*( * _{k}*)

*ij* *t*

ρ . The

theorem gives

*t* *t* *dV* *t _{k}*

_{ij}*t*

_{k}*dV*

*v*
*K*
*k*
*c*
*ij*
*k*
*ij*
*V*
*K*

*k* *ij* *k*

) ( ) ( ) ( ) ( 1 1 ε σ ε

σ Δ =_{∫ ∑} Δ

∫ ∑

=

= (12)

Where σ*ij*is given in Eq. (3). For the application of the von

Mises yield criterion, we have

*t* *t* *dV* _{ij}*t _{k}*

*dV*

*v*
*K*
*k* *y*
*k*
*ij*
*k*
*v*
*K*
*k*
*c*

*ij*( ) ( ) ( ( ))

1 1 ε ε σ ε

σ Δ =_{∫ ∑} Δ

∫ ∑

=

= (13)

∫ ∑ Δ

Δ +

∫∑ Δ −∫ ∑ +

=

=

= =

*V*
*K*
*k* *ij* *ij* *k*

*k*
*ij*
*k*
*r*
*ij*
*k*

*V* *k* *ij*

*K*

*k* *V*

*K*
*k*

*P*
*ij*
*k*

*ij*
*y*

*dV*
*t*

*dV*
*t*
*t*
*t*
*t*
*dV*

*t*

1

1 1

) (

) ( )) ( ) ( ) ( ( ))

( (

ε σ

ε ρ σ σ ε

ε σ λ

θ

(14)

where ε Δε*ij* *tk* = 3Δε*ij*Δε*ij*

2

)) (

( is the effective plastic strain

increment at *tk*. This multiplier λ gives the capacity of the

body subjected to cyclic loads *P*and θ to withstand constant

loads *P*and θ before ratchetting occurs. On the basis of this

formulation, the LMM produces a sequence of monotonically reducing upper bounds, which converges to the least upper bound ratchet limit for the chosen class of displacement fields. In the following sections, a symmetric cracked welded pipe is analysed in detail using the proposed method.

**PIPE GEOMETRY AND MATERIAL PROPERTIES **

Consider a circumferentially welded pipe, with a circumferential symmetric inner/central/outer surface crack in the weld (Fig. 1). The inhomogeneous pipe includes two different material domains - Parent Material (PM) and Weld Metal (WM). Each material is isotropic, elastic perfectly plastic and satisfies the von Mises yield criterion. The initial residual stress in the pipe due to the welding process is considered to be

ignored due to post weld heat treatment. The length *L*, inner

radius *Ri*, wall thickness *w*, crack length *a* and weld width

*H* are shown in Fig. 1 and Table 1. The material properties

including the yield stress σ*y*, Young’s modulus *E*, Poisson’s

ratio ν , conductivity *k* _{ and coefficient of thermal expansion }

α adopted in this paper for the baseline calculation are given in

Table 2, where WM and PM have same values of *E*, *k* and

ν .** **

**LOADING CONDITIONS AND FINITE ELEMENT **
**MODELLING **

In this analysis, the pipe is subjected to two loading

conditions: i) Δθ+*p*, a cyclic temperature Δθ and a constant

internal pressure *p* (with closed end conditions) (Fig. 2a) or

(ii) Δθ+*T* , a cyclic temperature Δθ and a constant axial

tension *T*(Fig. 2b).

Fig.1 Welded pipe configurations with (a) an inner surface crack, (b) a central crack and (c) an outer surface crack

Table 1 Shape parameters of a welded pipe with a symmetric crack

)
(*mm*

*w* *L* *Ri* *a* *H*

40 5*w* 7.5*w* 0.5*w* 0.5*w*

Table 2 Material properties of a welded pipe

*PM*
*y*

σ (MPa)

*WM*
*y*

σ (MPa)

*E*

(GPa)

*PM*

α

)
10
( −5o* _{C}*−1

*WM*

α

)
10
( −5o* _{C}*−1

*k*

) ( −1 −1

*C*
*Wm* o ν

230 460 200 1.9 1.8 15 0.3

Fig. 2 Thermal and mechanical loads and boundary conditions of the
cracked welded pipe: (a) Δθ+*p* or (b) Δθ+*T*

Fig. 2 shows the two-dimensional axisymmetric model, with a symmetry condition applied in the axial direction. The end of the pipe is constrained to remain in-plane, simulating the expansion of a long pipe. The closed end condition of the pipe is simulated by applying an equivalent axial tension

) 2

/( 2

2

*w*
*w*
*R*
*pR*

*q*= _{i}* _{i}* + .

It is assumed that the ambient air temperature outside of

the pipe is θ0, and the operating temperature of the fluid

contained within the pipe fluctuates between ambient and a

higher value, θ0+Δθ (Fig. 3). Due to the dissimilar material

in the pipe, the applied cyclic thermal loading may be constructed by three thermal stress extremes: i) a thermal stress field produced by a linear temperature gradient through the wall

Centre-line of weld

Centre-line of

th

e pip

e

### θ

### θ

0+Δ*T*

### )

### (

*b*

0

### θ

Centre-line

of

th

e

p

ip

e

### θ

### θ

0 +Δ*p*

### )

### (

*a*

*q*

Centre-line of weld

0

### θ

)
(*a*

Ce

n

tr

e

‐

line

o

f

the

pip

e

PM

WM

*L*
*H*

*a*

*i*

*R* *W*

)
(*b*

PM

WM
*a*

PM

WM
*a*

thickness; ii) a thermal stress field due to the different thermal expansion coefficients between the PM and WM occurring at the highest uniform temperature; and iii) a zero thermal stress

field simulating a uniform ambient temperature. If θ0 is zero,

the maximum effective elastic thermal stresses for these three extremes can be determined by the maximum temperature

difference Δθ . Hence the thermal load history can be

characterised byΔθ.

Fig. 3 The operating temperature history of the fluid contained within the welded pipe

Fig. 4 Finite element mesh of the welded pipe with an inner
crack*a*=0.5*w*

In this paper, the Abaqus type CAX8R 8-node biquadratic axisymmetric quadrilateral elements with reduced integration are used for structural analysis and DCAX8 8-node quadratic axisymmetric heat transfer quadrilateral elements with reduced integration scheme are used for the heat transfer analysis (Fig. 4).

**RESULTS AND DISCUSSIONS **

In this paper, a mismatch rate *r*in the yield stress between

the WM and the PM is introduced

*PM*

*y*
*WM*
*y*

*r*=σ /σ (15)

**Effect of crack location and yield stress of weld metal **

*WM*
*y*

σ ** on the ratchet limits **

In this subsection, pipes with inner/central/outer surface cracks in the weld are considered. The values of yield stress of

the WM *WM*

*y*

σ used are 115, 230 and 460MPa, respectively, and

*PM*
*y*

σ is held constant at 230MPa (i.e. *r*=0.5, 1 and 2).

Fig. 5 show the converged ratchet limit interaction curves

of cracked welded pipes with *r*=0.5, 1, 2 and a pure PM pipe

( *r*=1) without a crack, subjected to Δθ+*p* (Fig. 5a) or

*T*
+

Δθ (Fig. 5b). In this diagram, a normalised internal

pressure *p*/*pPM* (or axial tension *T*/*TPM* ) and a temperature

rangeΔθ are chosen as an abscissa and an ordinate respectively.

*PM*

*p* and *TPM* are the limit internal pressure and limit axial

tension of the pure PM pipe without a crack, respectively.

Fig. 5 Ratchet limit interaction curves of the welded pipe with the
different *r* and the different crack locations. The pipe is subjected to

(a) Δθ+*p* or (b) Δθ+*T*.

In the Fig. 5, it can be seen that only the ratchet limit boundaries of the pure PM pipe without a crack and the welded

pipe (*r*=2) with an inner/central/outer crack (excluding an

inner crack in Fig. 5b) exhibit typical Bree-like diagrams. The ratchet limit boundaries in other cases interacts the y-axis. For example, the point A in Fig. 5b represents a maximum temperature range to avoid ratchetting for an applied cyclic thermal load and a particular form of a potential mechanical load. The point B denotes the limit load for the applied mechanical load.

Fig. 5 shows that for all *r*, the three different locations of

the symmetric crack have little effect on the ratchet limit

boundaries, except for the case of *r*=2and Δθ ≥400o*C* in

0 100 200 300 400 500

0 0.2 0.4 0.6 0.8 1

outer inner central

2
=
*r*

1
=
*r*

5 . 0 =

*r*

pure PM pipe without crack crack position:

*PM*
*T*

*T*

)
(*b*

**A**

**B**

case**C**

case **D**

### )

### (

o*C*

### θ

### Δ

0 100 200 300 400 500

0 0.2 0.4 0.6 0.8 1

outer inner central

2
=
*r*

1

=
*r*

5 . 0 =

*r*

pure PM pipe without crack crack position:

*PM*
*p*

*p*

### )

### (

*a*

### )

### (

o*C*

### θ

### Δ

)
(*t*

θ

θ θ0+Δ

0

θ

*t*

2

*t*

1

Fig. 5b, where the inner surface crack produces much lower ratchet limits than the central crack and outer surface crack.

It can be observed that the ratchet limit boundaries including the limit internal pressure / axial tension and the maximum temperature range to avoid ratchetting reduce with

the decreasing *r*. It is also noted that for the case of Δθ+*p*,

when *r*≥1 and _{Δ}θ_{<}_{100}o*C*_{ ( Fig. 5a), the change in }_{r}_{ has little }

effect on the ratchet limit boundary due to the plastic collapse occurring in the PM.

Fig. 6 The non-ratchetting/ratchetting mechanisms for the inner cracked welded pipe (Fig. 5a) subjected to a cyclic temperature range

θ

Δ and a constant internal pressure ( *p*/*p _{PM}* =0.15), when (a)

2 =

*r* , _{Δ}θ_{=}_{500}o*C* _{ (no ratchetting mechanism), (b) }* _{r}*=

_{1}

_{, }

*C*

o 185 =

Δθ (ratchetting mechanism in WM) and (c) *r*=0.5 ,

*C*

o 88 =

Δθ (ratchetting mechanism in WM)

Fig. 7 Abaqus verification of the ratchet limit for the cyclic
temperature of Δθ=_{200}o*C*_{ using detailed step by step analysis }

Three typical failure modes are given in Fig. 6 which shows the non-ratchetting/ratchetting mechanisms for the inner cracked welded pipe (Fig. 5a), subjected to a cyclic temperature

range Δθ and a constant internal pressure ( *p*/*pPM* =0.15).

When *r*=2 and _{Δ}θ_{=}_{500}o*C*_{(}_{Fig. 6a}_{)}_{, no ratchetting mechanism }

occurs and the pipe still has a capacity to resist an additional

internal pressure. When *r*=1 , Δθ=88o*C* (Fig. 6b) or

5 . 0 =

*r* ,Δθ =185o*C*(Fig. 6c), a ratchetting mechanism occurs

at the weld material, and the pipe will experience incremental plastic collapse after a limited number of cycles.

It is particularly interesting that for the case of *r*=2, after

the pipe is subjected to the cyclic temperature range

*C*

o

470 ≥

Δθ , the pipe with an inner surface crack can

withstand an internal pressure but cannot withstand an axial tension. This is because the thermal stress in the plastic zone could be reduced by the superposition of the mechanical stress caused by an internal pressure, but not by an axial tension.

Consider two load cases C and D (Fig. 5b), which are just outside and inside the predicted ratchet limit domain at

temperature range Δθ_{=}_{200}o*C*_{. The plastic strain histories (Fig. }

7) calculated by the ABAQUS step-by-step analysis verified the accuracy of LMM ratchet limit boundary by showing that i) under the load case C, the maximum equivalent plastic strain increases with load cycles to give a strong ratchetting mechanism; and ii) under the load case D, the maximum equivalent plastic strain ceases to increase after 20 load cycles, giving a non-ratchetting mechanism.

**Effect of crack size **

Fig. 8 Ratchet limit interaction curves of the welded pipe with the
different crack sizes *a* and the different *r*. The pipe is subjected to
(a) Δθ+*p* or (b) Δθ+*T*

Three symmetric crack lengths are considered: *a*=0.25*w*,

*w*

5 .

0 and 0.75*w*. For each crack length, three yield stresses

are considered as per the previous sections, *r*=0.5, 1 and 2.

0 100 200 300 400 500

0 0.2 0.4 0.6 0.8 1

*PM*
*T*

*T*
2

=
*r*

1
=
*r*

5 . 0 =

*r*

pure PM pipe without crack

25 . 0

=
*w*
*a*

5 .

0 0.75

### )

### (

*b*

### )

### (

o*C*

### θ

### Δ

0 100 200 300 400 500

0 0.2 0.4 0.6 0.8 1

*PM*
*p*

*p*

### )

### (

*a*

2
=
*r*

1
=
*r*

5 . 0 =

*r*

pure PM pipe without crack

25 . 0

=
*w*
*a*

5 .

0 0.75

### )

### (

o*C*

### θ

### Δ

0 5 10 15 20 25

0 2 4 6 8 10 12 14 16 18 20 22 24

cyclic load case **C**

cyclic load case **D**

Number of cycles

Eq

uiv

al

e

n

t

p

la

st

ic

st

rai

n

crack )

(*a* (*b*) (*c*)

Failure pattern No failure

PM PM PM

Fig. 8 gives ratchet limit interaction curves of the pipe

subjected to Δθ+*p*(Fig. 8a) or Δθ+*T* (Fig. 8b). It shows that

i) when *r*≤1 (excluding the case of *r*=1 and *a*≤0.5*w*in Fig.

8a), the ratchet limit boundaries including the limit internal pressure / axial tension and the maximum temperature range to

avoid ratchetting reduces with the increasing *a*; ii) when *r*=2

and _{Δ}_{θ}_{<}_{300}o*C*_{ (except for the case of }* _{a}*=

_{0}

_{.}

_{75}

_{w}_{ in Fig. 8b), }

the change in *a* has little effect on the ratchet limit diagrams.

The reason of the reduction in the limit load with the increasing

*a* is due to the plastic collapse occurring in the WM. A larger

crack length in the WM causes a smaller effective load carrying area, which leads to a lower limit internal pressure / axial tension.

**Effect of weld width **

In order to study the effect of weld width, values of

*w*

*H* =0.25 , 0.5*w* and *w* were chosen. Similarly, all limits for

three different width are computed based on three different

yield stresses of WM: *r*=0.5, 1 and 2.

Fig. 9 Ratchet limit interaction curves of the pipe with the different
thickness*H* of the WM and the different *r*. The pipe is subjected to
(a) Δθ+*p* or (b) Δθ+*T*

Fig. 9 gives ratchet limit interaction curves of the pipe

subjected to Δθ+*p*(Fig. 9a) or Δθ+*T*(Fig. 9b). It shows that

for all *r*(excluding the cases of *r*=2 and *H* =0.25*w*), the

change in *H*has little effect on the ratchet limit diagrams.

Fig. 9b shows that when *r*=2, the width *H*=0.25*w*gives

a smaller limit tension than that of *H*=0.5*w* and *w*. This is

because the pipe failure zone is a 45 degree inclined strip which is from the crack tip to the side boundary. Hence, the smaller

width *H*of WM means that this 45 degree slip line must travel

further through weaker parent material, which causes the lower

limit tension of the pipe. The width *H*=0.25*w*also gives a

smaller maximum temperature range to avoid ratchetting than

that of *H* =0.5*w* and *w* due to the aforementioned reason.** **

**Effect of coefficient of thermal expansion of weld **
**metal **α*WM*_{ }

Three values of α*WM* α*PM* =0.5

, 0.95 and 2 were chosen. The thermal expansion of the PM material was given a fixed

value of α*PM* =1.8 5 1

10− −

× o*C* . All limits for the three

differentα*WM*

are computed based on three different yield

stresses of WM: *r*=0.5, 1 and 2.

** **

Fig. 10 Ratchet limit interaction curves of the pipe with the different
thermal expansion coefficients of the WM α*WM*

and the different *r*,
where α*PM* =1.9

( 5 1

10− −

× o*C* _{). The pipe is subjected to (a) }
*p*

+
Δθ or
(b) Δθ+*T*

Fig. 10 gives ratchet limit interaction curves of the pipe

subjected to Δθ+*p*(Fig. 10a) or Δθ+*T* (Fig. 10b). It shows

that for all *r*, i) the change in α*WM*

has no effect on the limit internal pressure (or limit axial tension) due to the purely

mechanical nature of the load; and ii) α*WM*/α*PM* =2

gives a

0 100 200 300 400 500

0 0.2 0.4 0.6 0.8 1

*PM*
*T*

*T*

2

=
*r*

1

=
*r*

5 . 0 =

*r*

pure PM pipe without crack

5
.
0
=
*PM*
*WM*
α
α

95 .

0 2

### )

### (

*b*

### )

### (

o*C*

### θ

### Δ

0 100 200 300 400 500

0 0.2 0.4 0.6 0.8 1

*PM*
*p*

*p*

)
(*a*

2

=
*r*

1

=
*r*

5 . 0 =

*r*

pure PM pipe without crack

5 . 0 =

*PM*
*WM*
α
α

95 .

0 2

### )

### (

o*C*

### θ

### Δ

0 100 200 300 400 500

0 0.2 0.4 0.6 0.8 1
*PM*
*T*

*T*

)
(*b*

2
=
*r*

1

=
*r*

5 . 0 =

*r*

pure PM pipe without crack

25 . 0 =

*w*
*H*

5 .

0 1

### )

### (

o*C*

### θ

### Δ

0 100 200 300 400 500

0 0.2 0.4 0.6 0.8 1

2
=
*r*

1

=
*r*

5 . 0 =

*r*

pure PM pipe without crack

25 . 0 =

*w*
*H*

5 .

0 1

*PM*
*p*

*p*

### )

### (

*a*

### )

### (

o*C*

### θ

smaller maximum temperature range to avoid ratchetting in

comparison with the cases of α*WM*/α*PM* =0.5

and 0.95. This is because a larger difference in thermal expansion coefficients between the PM and the WM leads to a larger field of high thermal stress around the interface between two materials, which may interact with the another high stress field either around the crack tip or in the parent material, thus causing failure at smaller temperature range.

**Discussions **

In the previous subsections, the results show that five

parameters -- the yield stress of WM *WM*

*y*

σ , the location

(inner/central/outer) and length *a* of the crack, the width

*w*and the thermal expansion coefficient α*WM*

of WM have the different effects on the ratchet limits, maximum temperature ranges to avoid ratchetting, and limit loads. Among these

parameters, *WM*

*y*

σ is the most sensitive parameter to the ratchet

limit boundary, and the crack location is the least sensitive one. A further investigation of the effect of these parameters is given in the Fig. 11 and Tables 3-6.

Fig. 11 shows how the yield stress of WM affects the ratchet limit of the pipe with an inner surface crack. It suggests that the higher WM yield strength leads to a larger limit load and a larger maximum temperature range to avoid ratchetting

for both loading cases. It is noted that for the case of Δθ+*p*,

there is a rapid increase in limit load up to *r*=0.75, with the

increases being small in comparison when *r*>0.75 (shown in

Fig. 11a). When *r*>1.5, the maximum temperature range to

avoid ratchetting steeply rises with the increasing *r*, shown in

Fig. 11b. All trend lines are fit to the data to give the functions, shown in Eqs. (16-19).

For the pipe subjected to Δθ+*p*, we have

⎩
⎨
⎧
≤
<
+
≤
≤
−
=
2
0.8
0.89
0.079
0.8
0.5
0.018
21
.
1
*r*
*r*
*r*
*r*
*p*
*p*
*PM*
(16)
⎪
⎪
⎩
⎪
⎪
⎨
⎧
≤
<
>
≤
<
+
≤
<
−
≤
≤
+
+
=
Δ
2
1.55
500
1.55
1.54
1.78
0.71
-1.54
1.5
1190
1000
1.5
0.5
52
14
.
33
42
.
91 2
*r*
*r*
*r*
*r*
*r*
*r*
*r*
*r*
*p*
θ
(17)

For the pipe subjected to Δθ+*T*

2 0.5 098 . 0 86 . 0 16 .

0 2+ − ≤ ≤

−

= *r* *r* *r*

*T*
*T*

*PM*

(18)

89.52 23.33 60 0.5 2

2+ − ≤ ≤

=

Δθ*T* *r* *r* *r*

(19)

where *pPM* and *TPM* are the limit internal pressure and limit

axial tension of the pure PM pipes without a crack,

respectively. Δθ*p*

or Δθ*T*

represents the maximum temperature range to avoid ratchetting for the pipe subjected to an applied

cyclic thermal load Δθand a potential internal pressure *p* or

axial tension *T*, respectively.

Fig. 11 The effect of the yield stress of WM *WM*
*y*

σ on (a) the limit loads
and (b) the maximum temperature ranges of the pipe under i) Δθ+*p*

or ii) Δθ+*T*

Table 3 Limit load and maximum temperature range of the pipe with
the different crack locations and the different *r*, where *a*/*w*=0.5,

5
.
0
/*w*=

*H* and α*WM*/α*PM* =0.95_{. The pipe is subjected to (a) }

*p*

+

Δθ or

(b) Δθ+*T*

Normalised limit load

*PM*
*p*

*p*/ (

*PM*
*T*

*T*/ )

Maximum temperature

range _{Δ}θ*p*

or _{Δ}θ*T*

(o*C*_{) }

Loading condition crack location 5 . 0 =

*r* *r*=1 *r*=2 *r*=0.5 *r*=1 *r*=2

inner 0.59 0.98 1.05 90 180 - outer 0.50 0.93 1.08 84 167 -

*p*

+ Δθ

central 0.54 0.99 1.08 95 190 -

inner 0.30 0.60 0.99 90 180 470 outer 0.29 0.58 0.95 84 167 -

*T*

+ Δθ

central 0.29 0.59 1.03 95 190 -

0 0.2 0.4 0.6 0.8 1 1.2

0.5 0.7 0.9 1.1 1.3 1.5 1.7 1.9 2.1

⎩
⎨
⎧
≤
<
+
≤
≤
−
=
2
0.8
0.89
0.079
0.8
0.5
0.018
21
.
1
*r*
*r*
*r*
*r*
*p*
*p*
*PM*
2
0.5
098
.
0
86
.
0
16
.

0 2_{+} _{−} _{≤} _{≤}

−

= *r* *r* *r*

*T*
*T*
*PM*

*r*

*PM*

*PM*

*T*

*T*

*p*

*p*,

limit pressure *p* trend
limit tension *T* trend

### )

### (

*a*

0
100
200
300
400
500
0.5 0.7 0.9 1.1 1.3 1.5 1.7 1.9 2.1

### ( )

*C*

*T*
*p*

### θ

o### θ

### Δ

### Δ

### ,

*r*

⎪
⎪
⎩
⎪
⎪
⎨
⎧
≤
<
>
≤
<
+
≤
<
−
≤
≤
+
+
=
Δ
2
1.55
500
1.55
1.54
1.78
0.71
-1.54
1.5
1190
1000
1.5
0.5
52
14
.
33
42
.
91 2
*r*

*r*

*r*

*r*

*r*

*r*

*r*

*r*

*P*θ 2 0.5 60 33 . 23 52 .

89 2_{+} _{−} _{≤} _{≤}

=

Δθ*T* *r* *r* *r*

Table 4 Limit load and maximum temperature range of the inner
cracked pipe with the different crack length *a* and the different *r*,
where*H*/*w*=0.5 and α*WM*/α*PM*=0.95_{. The pipe is subjected to (a) }

*p*

+

Δθ or (b) Δθ+*T*

Normalised limit load

*PM*
*p*

*p*/ (

*PM*
*T*

*T*/ )

Maximum temperature

range _{Δ}θ*p*

or _{Δ}θ*T*

(o*C*_{) }

Loading condition

crack size

*w*

*a*/ _{r}_{=}_{0}_{.}_{5}

1 =

*r* *r*=2 *r*=0.5 *r*=1 *r*=2
0.25 0.93 1.00 1.08 110 320 -
0.50 0.59 0.98 1.05 90 180 -

*p*

+ Δθ

0.75 0.30 0.60 0.94 60 130 270 0.25 0.48 0.89 1.03 110 360 - 0.50 0.30 0.60 0.99 90 180 470

*T*

+ Δθ

0.75 0.15 0.31 0.61 60 120 270

Table 5 Limit load and maximum temperature range of the inner
cracked pipe with the different thickness of the WM *H*and the
different *r*, where *a*/*w*=0.5and α*WM*/α*PM*=0.95_{. The pipe is }

subjected to (a) Δθ+*p* or (b) Δθ+*T*

Normalised limit load

*PM*
*p*

*p*/ (*T*/*T _{PM}*)

Maximum temperature
range Δθ*p*

or Δθ*T*

(o*C*_{) }

Loading condition

WM width

*w*
*H*/

5 . 0

=

*r* *r*=1 *r*=2 *r*=0.5 *r*=1 *r*=2

0.25 0.72 0.98 1.02 90 180 420

0.5 0.59 0.98 1.05 90 180 -

*p*

+ Δθ

1 0.59 0.98 1.09 80 160 -

0.25 0.37 0.60 0.84 90 180 300

0.5 0.30 0.60 0.99 90 180 470

*T*

+ Δθ

1 0.30 0.60 1.05 80 160 -

Table 6 Limit load and maximum temperature range of the inner
cracked pipe with the different α*WM*_{and the different }_{r}_{, where }

9 . 1

=

*PM*

α ( 5 1

10− −

× o*C* ), *a*/*w*=0.5 and *H*/*w*=0.5. The pipe is
subjected to (a) Δθ+*p* or (b) Δθ+*T*

Normalised limit load

*PM*
*p*

*p*/ (*T*/*T _{PM}*)

Maximum temperature
range _{Δ}θ*p*

or _{Δ}θ*T*

(o*C*_{) }

Loading condition

*PM*
*WM* α
α /

5 . 0 =

*r* *r*=1 *r*=2 *r*=0.5 *r*=1 *r*=2

0.5 0.59 0.98 1.05 100 200 470

0.95 0.59 0.98 1.05 90 180 -

*p*

+ Δθ

2 0.59 0.98 1.05 52 110 220

0.5 0.30 0.60 0.99 100 200 410

0.95 0.30 0.60 0.99 90 180 470

*T*

+ Δθ

2 0.30 0.60 0.99 52 110 210

The obtained results are further summarised in Tables 3-6 which show the effects of the crack location, crack length, weld width and weld thermal expansion coefficient on the limit load and maximum temperature range to avoid ratchetting, respectively. The conclusion is given in next section.

**CONCLUSION **

The extended Linear Matching Method (LMM) is successfully applied in this study for the ratchet limit analysis of circumferentially welded pipes containing a circumferential

crack subjected to a cyclic temperature Δθ and a constant i)

internal pressure *p* or ii) axial tension *T* . Based on the results

obtained in this study, the following conclusions are given: i) When compared with a pure Parent Material (PM) pipe without a crack, the discontinuity in material (due to the Weld Metal (WM)) and in geometry (due to a crack) may lead to a significant change in the ratchet limit boundary including the maximum temperature range to avoid ratchetting and limit load; ii) Among five parameters, variation of the yield stress

*WM*
*y*

σ of the WM has the largest impact on the ratchet limits. The

limit load and the maximum temperature range to avoid

ratchetting rise with the increasing *WM*

*y*

σ . The relationship

between them has been formulated; iii) An increase in the

symmetric crack length *a*decreases the maximum temperature

range to avoid ratchetting and limit load, but the crack location has the least effect on the ratchet limit out of the parameters

considered in this work; iv) The weld width *H*has little effect

on the limits for all *r* , except for the case of *r*=2and

*w*

*H*=0.25 when the pipe is under axial tension, where the

ratchet limit boundary is significantly reduced in comparison

with cases of *r*=2 and *H*≥0.5*w*; v) The large difference in

the coefficient of thermal expansion between the WM and the PM significantly decreases the maximum temperature ranges to avoid ratchetting, but the limit load is unaffected by any

changes in α*WM* α*PM*

/ .

**ACKNOWLEDGEMENTS **

The authors gratefully acknowledge the support of the Engineering and Physical Sciences Research Council of the United Kingdom, and the University of Strathclyde during the course of this work.

**REFERENCES **

[1] Brickstad, B., and Josefson, B.L., 1998, “A parameter study of residual stress in multi-pass butt-welded stainless steel pipes”, International Journal of Pressure Vessels and Piping, 75, pp.11-25.

[2] Roos, E., Schuler, X., and Stumpfrock, L., July 26-30 2009, “Numerical evaluation of ratchetting effect on the deformation and failure behaviour of components”, Proceedings of the ASME 2009 pressure vessels and piping division conference, Prague, Czech Republic.

[3] Carter, P., 2005, “Analysis of cyclic creep and rupture”. Part 1: boundary theorems and cyclic reference stress. International Journal of Pressure Vessels and Piping, 82, pp.15-26.

[4] Bree, J., 1989, “Plastic deformation of a closed tube due to interaction of pressure stresses and cyclic thermal stresses”. International Journal of Mechanical Sciences,; 31(11-12), pp.865-892.

[5] Koiter, W.T., 1960, “General theorems for elastic plastic solids”. Progress in solid mechanics, Sneddon JN and Hill R, eds., North Holland, Amsterdam, 1, pp.167-221.

[6] Melan, E., 1936, “Theorie statisch unbestimmter systeme aus ideal-plastichem baustoff”. Sitzungsber. d. Akad. d. Wiss., Wien 2A 145, pp.195–218.

[7] Muscat, M., Mackenzie, D., and Hamilton, R., 2003, “Evaluating shakedown by non-linear static analysis”. Computers and Structures, 81, pp.1727-1737.

[9] Staat, M., and Heitzer, M., 2001, “LISA a European project for FEM-based limit and shakedown analysis”. Nuclear Engineering and Design, 206, pp.151-166.

[10] Seshadri, R., 1995, “Inelastic evaluation of mechanical and structural components using the generalized local stress strain method of analysis”. Nuclear Engineering and Design, 153(2-3), pp.287-303.

[11] Mackenzie, D., Boyle, J.T., Hamilton, R., and Shi, J., 1996, “Elastic compensation method in shell-based design by analysis”. Proceedings of the 1996 ASME Pressure Vessels and

Piping Conference, 338**, **pp**.**203-208.

[12] Mackenzie, D., Boyle, J.T., and Hamilton, R., 2000, “The elastic compensation method for limit and shakedown analysis: a review”. Trans IMechE, Journal of Strain Analysis for Engineering Design, 35(3), pp.171-188.

[13] Chen, H.F., and Ponter, A.R.S., 2001, “Shakedown and limit analyses for 3-D structures using the Linear Matching Method”. International Journal of Pressure Vessels and Piping, 78, pp.443–451.

[14] Chen, H.F., and Ponter, A.R.S., 2005, “Integrity assessment of a 3D tubeplate using the linear matching method”. Part 1. Shakedown, reverse plasticity and ratchetting, International Journal of Pressure Vessels and Piping, 82(2), pp.85-94.

[15] Ponter, A.R.S., and Chen, H.F., 2001, “A minimum theorem for cyclic loading in excess of shakedown, with applications to the evaluation of a ratchet limit”. European Journal of Mechanics A/Solids, 20, pp. 539-554.

[16] Chen, H.F., and Ponter, A.R.S., 2001, “A method for the evaluation of a ratchet limit and the amplitude of plastic strain for bodies subjected to cyclic loading”. European Journal of Mechanics, A/Solids, 20(4), pp.555-571.

[17] Chen, H.F., and Ponter, A.R.S., 2006, “Linear Matching Method on the evaluation of plastic and creep behaviours for bodies subjected to cyclic thermal and mechanical loading”. International Journal for Numerical Methods in Engineering, 68, pp.13-32.

[18] Chen, H.F., 2010, “A direct method on the evaluation of ratchet limit”. Journal of Pressure Vessel Technology. 132, 041202.

[19] Chen, H.F., Ponter, A.R.S., and Ainsworth, R.A., 2006, “The Linear Matching Method applied to the high temperature life integrity of structures”, Part 1: Assessments involving constant residual stress fields. International Journal of Pressure Vessels and Piping, 83(2), pp.123-135.

[20] Chen, H.F., Ponter, A.R.S., and Ainsworth, R.A., 2006, “The Linear Matching Method applied to the high temperature life integrity of structures”, Part 2: Assessments beyond shakedown involving changing residual stress fields. International Journal of Pressure Vessels and Piping, 83(2),